 frequency at which occurs  frequency at which n measured. 0.01. E gap. E gap. Charge Carrier Related Nonlinearities. Bandgap Renormalization (Band Filling). Absorption induced transition of an electron from valence to conduction band conserves k x,y !.
Download Policy: Content on the Website is provided to you AS IS for your information and personal use and may not be sold / licensed / shared on other websites without getting consent from its author.While downloading, if for some reason you are not able to download a presentation, the publisher may have deleted the file from their server.
0.01
Egap
Egap
Charge Carrier Related Nonlinearities
Bandgap Renormalization (Band Filling)
Absorption induced transition
of an electron from valence to
conduction band conserves kx,y!
Conduction Band
Valence Band
Before Absorption
After Absorption
Egap
Egap>Egap
Egap
Recombination
time
KramersKronig
ky
E
kx
ExcitonBleaching
Charge Carrier Nonlinearities Near Resonance
“Transparency point”
Gain
0
Loss


Active Nonlinearities (with Gain)
Optical or
electrical
pumping
Stimulated
emission
Get BOTH an index
change AND gain!
KramersKrönig used to calculate
index change n() from ().
Ultrafast Nonlinearities Near Transparency Point
At the transparency point, the losses are balanced by
gain so that carrier generation by absorption is no
longer the dominant nonlinear mechanism for
index change. Of course one gets the Kerr effect +
other psand subpsphenomena which now dominate.
Evolution of carrier density in time
“Spectral Hole Burning”
“hole” in conduction band due to
to stimulated emission at maximum
gain determined by maximum
product of the density of occupied
states in conduction band and
density of unoccupied states in
valence band
“Carrier Heating”
(Temperature Relaxation)
electron collisions return carrier
distribution to a Fermi distribution
at a lower electron temperature
SHB – Spectral Hole Burning
Experiments have confirmed these calculations!
Semiconductor Response for Photon Energies Below the Bandgap
As the photon frequency decreases away from the bandgap, the contribution to the electron
population in the conduction band due to absorption decreases rapidly. Thus other mechanisms become important. For photon energies less than the band gap energy, a number of passive ultrafast nonlinear mechanisms contribute to n2 and 2. The theory for the Kerr effect is based on single valence and conduction bands with the electromagnetic field altering the energies of both the electrons and “holes”.
There are four processes which contribute, namely the Kerr Effect, the Raman
effect (RAM), the Linear Stark Effect (LSE) and the Quadratic (QSE) Stark Effect. Shown
schematically below are the three most important ones.
The theoretical approach is to calculate first the nonlinear
absorption and then to use the KramersKronig
Relation to calculate the nonlinear index change .
 frequency at which occurs
 frequency at which n calculated
Kerr
Here Ep (“Kane energy”) and the constant Kare
given in terms of the semiconductor’s properties.
K=3100 cm GW1 eV5/2
QSE
Kerr
Quantum Confined Semiconductors
When the translational degrees of freedom of electrons in both the valence and conduction bands
are confined to distances of the order of the exciton Bohr radius aB, the oscillator strength is
redistributed, the bandgap increases, the density of states e(E) changes and new bound states
appear. As a result the nonlinear optical
properties can be enhanced or reduced)
in some spectral regions.
Quantum Wells
Absorption edge moves
to higher energies.
Multiple welldefined
absorption peaks due to
transitions between
confined states
Enhanced absorption
spectrum near band edge
Example of MultiQuantum Well (MQW) Nonlinearities
Index change per
excited electron
A factor of 34 enhancement!!
Quantum Dots
Quantum dot effects become important when the
crystallite size r0 aB (exciton Bohr radius). For example, the exciton Bohr radius for
CdSaB = 3.2nm, CdSeaB = 5.6nm, CdTeaB = 7.4nm and GaAsaB = 12.5nm.
Definitive measurements were performed
on very wellcharacterized samples by
Banfi. De Giorgio et al. in range aBr0 3aB
Measurements at1.2m (), 1.4m () and
1.58m () for CdTe
Measurements at 0.79m (+) for CdS0.9Se0.1
Note the trend that Im{(3)} seems to fall
when aBr0 !
Nonlinear Refraction and Absorption in Quantum Dots for aBr0 3aB:
IIVI Semiconductors
Experimental QD test of the previously discussed offresonance universal F2(x,x) and G2(x,x) functions for bulk semiconductors (discussed previously) by M. SheikBahae, et. al., IEEE J. Quant. Electron. 30, 249 (1994).
2
1018
0
0.7
0.5
0.6
0.8
1019
Real{(3)} in units of 1019m2V2
2
(/0)4Imag{(3)} in units of m2V2
1020
Bulk
CdS 0.69m
▼ CdTe 12, 1.4, 1.58m
4
1021
2.0
1.5
1.0
To within the experimental uncertainty (factor of 2), no enhancements were
found in IIVI semiconductors for the far offresonance nonlinearities!